# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2014

#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_EuIrIn4

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            EuIrIn4
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Eu In4 Ir'
_chemical_formula_weight         803.44

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
In In -0.7276 1.3100 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ir Ir -1.4442 7.9887 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   Cmcm

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z-1/2'
'x, -y, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z-1/2'
'x+1/2, -y+1/2, z-1/2'
'-x+1/2, y+1/2, z'

_cell_length_a                   4.5619(8)
_cell_length_b                   17.059(2)
_cell_length_c                   7.3056(12)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     568.54(16)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    1276
_cell_measurement_theta_min      2.4
_cell_measurement_theta_max      24.0

_exptl_crystal_description       rod
_exptl_crystal_colour            metallic
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.07
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    9.387
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1344
_exptl_absorpt_coefficient_mu    49.967
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_correction_T_min  0.000
_exptl_absorpt_correction_T_max  0.000
_exptl_absorpt_process_details   ?

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            1276
_diffrn_reflns_av_R_equivalents  0.0539
_diffrn_reflns_av_sigmaI/netI    0.0422
_diffrn_reflns_limit_h_min       -2
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_theta_min         2.39
_diffrn_reflns_theta_max         23.97
_reflns_number_total             279
_reflns_number_gt                278
_reflns_threshold_expression     >2σ(I)

_computing_data_collection       'SMART APEX II (Bruker,2010)'
_computing_cell_refinement       'SMART APEX II'
_computing_data_reduction        'SAINT (Bruker,2000)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_molecular_graphics    'Ortep-3v2 for windows (Farrugia, 1997)'
_computing_publication_material  'PLATON (Spek, 2008)'

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2σ(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0816P)²+34.8110P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    .
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.0014(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         279
_refine_ls_number_parameters     24
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0453
_refine_ls_R_factor_gt           0.0453
_refine_ls_wR_factor_ref         0.1194
_refine_ls_wR_factor_gt          0.1193
_refine_ls_goodness_of_fit_ref   1.164
_refine_ls_restrained_S_all      1.164
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Eu1 Eu 0.0000 0.37480(10) 0.2500 0.0130(7) Uani 1 4 d S . .
Ir1 Ir 0.0000 0.71906(7) 0.2500 0.0119(6) Uani 1 4 d S . .
In1 In 0.0000 0.18587(9) 0.0448(2) 0.0112(7) Uani 1 2 d S . .
In2 In 0.0000 0.56541(14) 0.2500 0.0159(8) Uani 1 4 d S . .
In3 In 0.0000 0.0000 0.0000 0.0177(8) Uani 1 4 d S . .


_geom_special_details            
;
 All s.u.'s (except the s.u. in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell s.u.'s are taken
 into account individually in the estimation of s.u.'s in distances, angles
 and torsion angles; correlations between s.u.'s in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell s.u.'s is used for estimating s.u.'s involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Eu1 In2 3.252(3) . ?
Eu1 In1 3.3035(13) 13_455 ?
Eu1 In1 3.3035(13) 6 ?
Eu1 In1 3.3035(13) 6_455 ?
Eu1 In1 3.3035(13) 13 ?
Eu1 Ir1 3.5015(15) 5_445 ?
Eu1 Ir1 3.5015(15) 5_545 ?
Eu1 In1 3.554(2) . ?
Eu1 In1 3.554(2) 10_556 ?
Eu1 In3 3.6194(10) 6 ?
Eu1 In3 3.6194(10) 5 ?
Eu1 In3 3.6194(10) 5_455 ?
Ir1 In2 2.621(3) . ?
Ir1 In1 2.6961(17) 2_565 ?
Ir1 In1 2.6961(17) 9_565 ?
Ir1 In1 2.7875(11) 5_455 ?
Ir1 In1 2.7875(11) 14_556 ?
Ir1 In1 2.7875(11) 5 ?
Ir1 In1 2.7875(11) 14_456 ?
Ir1 Eu1 3.5015(15) 5 ?
Ir1 Eu1 3.5015(15) 5_455 ?
In1 Ir1 2.6961(17) 9_565 ?
In1 Ir1 2.7875(10) 5_545 ?
In1 Ir1 2.7875(10) 5_445 ?
In1 In1 2.998(3) 10_556 ?
In1 In3 3.1877(17) . ?
In1 In1 3.228(2) 13 ?
In1 In1 3.228(2) 13_455 ?
In1 Eu1 3.3035(13) 13_455 ?
In1 Eu1 3.3035(13) 13 ?
In2 In3 3.1279(9) 5_455 ?
In2 In3 3.1279(9) 6 ?
In2 In3 3.1279(9) 6_455 ?
In2 In3 3.1279(9) 5 ?
In2 Eu1 3.7926(10) 9_566 ?
In2 Eu1 3.7926(10) 9_565 ?
In3 In2 3.1279(9) 13_455 ?
In3 In2 3.1279(9) 5_545 ?
In3 In2 3.1279(9) 13 ?
In3 In2 3.1279(9) 5_445 ?
In3 In1 3.1877(17) 9 ?
In3 Eu1 3.6194(10) 13 ?
In3 Eu1 3.6194(10) 13_455 ?
In3 Eu1 3.6194(10) 5_445 ?
In3 Eu1 3.6194(10) 5_545 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
In2 Eu1 In1 108.26(4) . 13_455 ?
In2 Eu1 In1 108.26(4) . 6 ?
In1 Eu1 In1 143.48(7) 13_455 6 ?
In2 Eu1 In1 108.26(4) . 6_455 ?
In1 Eu1 In1 81.38(5) 13_455 6_455 ?
In1 Eu1 In1 87.34(4) 6 6_455 ?
In2 Eu1 In1 108.26(4) . 13 ?
In1 Eu1 In1 87.34(4) 13_455 13 ?
In1 Eu1 In1 81.38(5) 6 13 ?
In1 Eu1 In1 143.48(7) 6_455 13 ?
In2 Eu1 Ir1 139.35(2) . 5_445 ?
In1 Eu1 Ir1 46.57(3) 13_455 5_445 ?
In1 Eu1 Ir1 102.24(4) 6 5_445 ?
In1 Eu1 Ir1 46.57(3) 6_455 5_445 ?
In1 Eu1 Ir1 102.24(4) 13 5_445 ?
In2 Eu1 Ir1 139.35(2) . 5_545 ?
In1 Eu1 Ir1 102.24(4) 13_455 5_545 ?
In1 Eu1 Ir1 46.57(3) 6 5_545 ?
In1 Eu1 Ir1 102.24(4) 6_455 5_545 ?
In1 Eu1 Ir1 46.57(3) 13 5_545 ?
Ir1 Eu1 Ir1 81.30(4) 5_445 5_545 ?
In2 Eu1 In1 155.06(3) . . ?
In1 Eu1 In1 56.01(4) 13_455 . ?
In1 Eu1 In1 89.48(4) 6 . ?
In1 Eu1 In1 89.48(4) 6_455 . ?
In1 Eu1 In1 56.01(4) 13 . ?
Ir1 Eu1 In1 46.53(2) 5_445 . ?
Ir1 Eu1 In1 46.53(2) 5_545 . ?
In2 Eu1 In1 155.06(3) . 10_556 ?
In1 Eu1 In1 89.48(4) 13_455 10_556 ?
In1 Eu1 In1 56.01(4) 6 10_556 ?
In1 Eu1 In1 56.01(4) 6_455 10_556 ?
In1 Eu1 In1 89.48(4) 13 10_556 ?
Ir1 Eu1 In1 46.53(2) 5_445 10_556 ?
Ir1 Eu1 In1 46.53(2) 5_545 10_556 ?
In1 Eu1 In1 49.89(5) . 10_556 ?
In2 Eu1 In3 53.84(2) . 6 ?
In1 Eu1 In3 161.62(5) 13_455 6 ?
In1 Eu1 In3 54.60(3) 6 6 ?
In1 Eu1 In3 106.92(3) 6_455 6 ?
In1 Eu1 In3 94.52(2) 13 6 ?
Ir1 Eu1 In3 149.120(17) 5_445 6 ?
Ir1 Eu1 In3 92.132(16) 5_545 6 ?
In1 Eu1 In3 138.41(2) . 6 ?
In1 Eu1 In3 108.80(2) 10_556 6 ?
In2 Eu1 In3 53.84(2) . 5 ?
In1 Eu1 In3 106.92(3) 13_455 5 ?
In1 Eu1 In3 94.52(2) 6 5 ?
In1 Eu1 In3 161.62(5) 6_455 5 ?
In1 Eu1 In3 54.60(3) 13 5 ?
Ir1 Eu1 In3 149.120(17) 5_445 5 ?
Ir1 Eu1 In3 92.132(16) 5_545 5 ?
In1 Eu1 In3 108.80(2) . 5 ?
In1 Eu1 In3 138.41(2) 10_556 5 ?
In3 Eu1 In3 60.61(2) 6 5 ?
In2 Eu1 In3 53.84(2) . 5_455 ?
In1 Eu1 In3 54.60(3) 13_455 5_455 ?
In1 Eu1 In3 161.62(5) 6 5_455 ?
In1 Eu1 In3 94.52(2) 6_455 5_455 ?
In1 Eu1 In3 106.92(3) 13 5_455 ?
Ir1 Eu1 In3 92.132(16) 5_445 5_455 ?
Ir1 Eu1 In3 149.120(17) 5_545 5_455 ?
In1 Eu1 In3 108.80(2) . 5_455 ?
In1 Eu1 In3 138.41(2) 10_556 5_455 ?
In3 Eu1 In3 107.67(4) 6 5_455 ?
In3 Eu1 In3 78.13(3) 5 5_455 ?
In2 Ir1 In1 126.98(4) . 2_565 ?
In2 Ir1 In1 126.98(4) . 9_565 ?
In1 Ir1 In1 106.04(8) 2_565 9_565 ?
In2 Ir1 In1 78.28(4) . 5_455 ?
In1 Ir1 In1 123.49(3) 2_565 5_455 ?
In1 Ir1 In1 72.10(4) 9_565 5_455 ?
In2 Ir1 In1 78.28(4) . 14_556 ?
In1 Ir1 In1 72.10(4) 2_565 14_556 ?
In1 Ir1 In1 123.49(3) 9_565 14_556 ?
In1 Ir1 In1 156.56(8) 5_455 14_556 ?
In2 Ir1 In1 78.28(4) . 5 ?
In1 Ir1 In1 123.49(3) 2_565 5 ?
In1 Ir1 In1 72.10(4) 9_565 5 ?
In1 Ir1 In1 109.83(6) 5_455 5 ?
In1 Ir1 In1 65.06(6) 14_556 5 ?
In2 Ir1 In1 78.28(4) . 14_456 ?
In1 Ir1 In1 72.10(4) 2_565 14_456 ?
In1 Ir1 In1 123.49(3) 9_565 14_456 ?
In1 Ir1 In1 65.06(6) 5_455 14_456 ?
In1 Ir1 In1 109.83(6) 14_556 14_456 ?
In1 Ir1 In1 156.56(8) 5 14_456 ?
In2 Ir1 Eu1 139.35(2) . 5 ?
In1 Ir1 Eu1 62.85(3) 2_565 5 ?
In1 Ir1 Eu1 62.85(3) 9_565 5 ?
In1 Ir1 Eu1 133.40(4) 5_455 5 ?
In1 Ir1 Eu1 67.73(4) 14_556 5 ?
In1 Ir1 Eu1 67.73(4) 5 5 ?
In1 Ir1 Eu1 133.40(4) 14_456 5 ?
In2 Ir1 Eu1 139.35(2) . 5_455 ?
In1 Ir1 Eu1 62.85(3) 2_565 5_455 ?
In1 Ir1 Eu1 62.85(3) 9_565 5_455 ?
In1 Ir1 Eu1 67.73(4) 5_455 5_455 ?
In1 Ir1 Eu1 133.40(4) 14_556 5_455 ?
In1 Ir1 Eu1 133.40(4) 5 5_455 ?
In1 Ir1 Eu1 67.73(4) 14_456 5_455 ?
Eu1 Ir1 Eu1 81.30(4) 5 5_455 ?
Ir1 In1 Ir1 107.90(4) 9_565 5_545 ?
Ir1 In1 Ir1 107.90(4) 9_565 5_445 ?
Ir1 In1 Ir1 109.83(6) 5_545 5_445 ?
Ir1 In1 In1 143.02(4) 9_565 10_556 ?
Ir1 In1 In1 57.47(3) 5_545 10_556 ?
Ir1 In1 In1 57.47(3) 5_445 10_556 ?
Ir1 In1 In3 121.08(6) 9_565 . ?
Ir1 In1 In3 104.91(4) 5_545 . ?
Ir1 In1 In3 104.91(4) 5_445 . ?
In1 In1 In3 95.90(3) 10_556 . ?
Ir1 In1 In1 55.26(5) 9_565 13 ?
Ir1 In1 In1 52.64(3) 5_545 13 ?
Ir1 In1 In1 123.35(9) 5_445 13 ?
In1 In1 In1 101.71(6) 10_556 13 ?
In3 In1 In1 130.80(5) . 13 ?
Ir1 In1 In1 55.26(5) 9_565 13_455 ?
Ir1 In1 In1 123.35(9) 5_545 13_455 ?
Ir1 In1 In1 52.64(3) 5_445 13_455 ?
In1 In1 In1 101.71(6) 10_556 13_455 ?
In3 In1 In1 130.80(5) . 13_455 ?
In1 In1 In1 89.93(8) 13 13_455 ?
Ir1 In1 Eu1 70.59(4) 9_565 13_455 ?
Ir1 In1 Eu1 168.30(5) 5_545 13_455 ?
Ir1 In1 Eu1 81.33(2) 5_445 13_455 ?
In1 In1 Eu1 130.69(2) 10_556 13_455 ?
In3 In1 Eu1 67.75(4) . 13_455 ?
In1 In1 Eu1 124.61(8) 13 13_455 ?
In1 In1 Eu1 65.93(5) 13_455 13_455 ?
Ir1 In1 Eu1 70.59(4) 9_565 13 ?
Ir1 In1 Eu1 81.33(2) 5_545 13 ?
Ir1 In1 Eu1 168.30(5) 5_445 13 ?
In1 In1 Eu1 130.69(2) 10_556 13 ?
In3 In1 Eu1 67.75(4) . 13 ?
In1 In1 Eu1 65.93(5) 13 13 ?
In1 In1 Eu1 124.61(8) 13_455 13 ?
Eu1 In1 Eu1 87.34(4) 13_455 13 ?
Ir1 In1 Eu1 77.97(4) 9_565 . ?
Ir1 In1 Eu1 65.74(4) 5_545 . ?
Ir1 In1 Eu1 65.74(4) 5_445 . ?
In1 In1 Eu1 65.06(3) 10_556 . ?
In3 In1 Eu1 160.95(5) . . ?
In1 In1 Eu1 58.06(5) 13 . ?
In1 In1 Eu1 58.06(5) 13_455 . ?
Eu1 In1 Eu1 123.99(4) 13_455 . ?
Eu1 In1 Eu1 123.99(4) 13 . ?
Ir1 In2 In3 110.90(4) . 5_455 ?
Ir1 In2 In3 110.90(4) . 6 ?
In3 In2 In3 138.20(8) 5_455 6 ?
Ir1 In2 In3 110.90(4) . 6_455 ?
In3 In2 In3 71.45(3) 5_455 6_455 ?
In3 In2 In3 93.64(4) 6 6_455 ?
Ir1 In2 In3 110.90(4) . 5 ?
In3 In2 In3 93.64(4) 5_455 5 ?
In3 In2 In3 71.45(3) 6 5 ?
In3 In2 In3 138.20(8) 6_455 5 ?
Ir1 In2 Eu1 180.0 . . ?
In3 In2 Eu1 69.10(4) 5_455 . ?
In3 In2 Eu1 69.10(4) 6 . ?
In3 In2 Eu1 69.10(4) 6_455 . ?
In3 In2 Eu1 69.10(4) 5 . ?
Ir1 In2 Eu1 74.40(4) . 9_566 ?
In3 In2 Eu1 131.174(11) 5_455 9_566 ?
In3 In2 Eu1 62.196(15) 6 9_566 ?
In3 In2 Eu1 62.196(15) 6_455 9_566 ?
In3 In2 Eu1 131.174(11) 5 9_566 ?
Eu1 In2 Eu1 105.60(4) . 9_566 ?
Ir1 In2 Eu1 74.40(4) . 9_565 ?
In3 In2 Eu1 62.196(15) 5_455 9_565 ?
In3 In2 Eu1 131.174(11) 6 9_565 ?
In3 In2 Eu1 131.174(11) 6_455 9_565 ?
In3 In2 Eu1 62.196(15) 5 9_565 ?
Eu1 In2 Eu1 105.60(4) . 9_565 ?
Eu1 In2 Eu1 148.79(8) 9_566 9_565 ?
In2 In3 In2 180.00(8) 13_455 5_545 ?
In2 In3 In2 93.64(4) 13_455 13 ?
In2 In3 In2 86.36(4) 5_545 13 ?
In2 In3 In2 86.36(4) 13_455 5_445 ?
In2 In3 In2 93.64(4) 5_545 5_445 ?
In2 In3 In2 180.0 13 5_445 ?
In2 In3 In1 65.49(4) 13_455 9 ?
In2 In3 In1 114.51(4) 5_545 9 ?
In2 In3 In1 65.49(4) 13 9 ?
In2 In3 In1 114.51(4) 5_445 9 ?
In2 In3 In1 114.51(4) 13_455 . ?
In2 In3 In1 65.49(4) 5_545 . ?
In2 In3 In1 114.51(4) 13 . ?
In2 In3 In1 65.49(4) 5_445 . ?
In1 In3 In1 180.000(6) 9 . ?
In2 In3 Eu1 112.05(2) 13_455 13 ?
In2 In3 Eu1 67.95(2) 5_545 13 ?
In2 In3 Eu1 57.06(5) 13 13 ?
In2 In3 Eu1 122.94(5) 5_445 13 ?
In1 In3 Eu1 122.35(3) 9 13 ?
In1 In3 Eu1 57.65(3) . 13 ?
In2 In3 Eu1 57.06(5) 13_455 13_455 ?
In2 In3 Eu1 122.94(5) 5_545 13_455 ?
In2 In3 Eu1 112.05(2) 13 13_455 ?
In2 In3 Eu1 67.95(2) 5_445 13_455 ?
In1 In3 Eu1 122.35(3) 9 13_455 ?
In1 In3 Eu1 57.65(3) . 13_455 ?
Eu1 In3 Eu1 78.13(3) 13 13_455 ?
In2 In3 Eu1 67.95(2) 13_455 5_445 ?
In2 In3 Eu1 112.05(2) 5_545 5_445 ?
In2 In3 Eu1 122.94(5) 13 5_445 ?
In2 In3 Eu1 57.06(5) 5_445 5_445 ?
In1 In3 Eu1 57.65(3) 9 5_445 ?
In1 In3 Eu1 122.35(3) . 5_445 ?
Eu1 In3 Eu1 180.00(4) 13 5_445 ?
Eu1 In3 Eu1 101.87(3) 13_455 5_445 ?
In2 In3 Eu1 122.94(5) 13_455 5_545 ?
In2 In3 Eu1 57.06(5) 5_545 5_545 ?
In2 In3 Eu1 67.95(2) 13 5_545 ?
In2 In3 Eu1 112.05(2) 5_445 5_545 ?
In1 In3 Eu1 57.65(3) 9 5_545 ?
In1 In3 Eu1 122.35(3) . 5_545 ?
Eu1 In3 Eu1 101.87(3) 13 5_545 ?
Eu1 In3 Eu1 180.00(4) 13_455 5_545 ?
Eu1 In3 Eu1 78.13(3) 5_445 5_545 ?

_diffrn_measured_fraction_theta_max 1.000
_diffrn_reflns_theta_full        23.97
_diffrn_measured_fraction_theta_full 1.000
_refine_diff_density_max         5.741
_refine_diff_density_min         -2.597
_refine_diff_density_rms         0.810
_database_code_depnum_ccdc_archive 'CCDC 988634'
